This book explains the observed trends in the bonding and structure of molecules and solids within the models of the ele
191 32 11MB
English Pages 272 [269] Year 1995
Bonding and Structure of Molecules and Solids D. G. PETTI FOR Isaac Wolfson Professor of Metallurgy Department of Materials University of Oxford
CLARENDON PRESS . OXFORD 1995
Oxford University Press, Walton Street, Oxford OX2 6DP Oxford New York Athens Auckland Bangkok Bombay Calcutta Cape Town Dar es Salaam Delhi Florence Hong Kong Istanbul Karachi Kuala Lumpur Madras Madrid Melbourne Mexico City Nairobi Paris Singapore Taipei Tokyo Toronto and associated companies in Berlin Ibadan Oxford is a trade mark of Oxford University Press Published in the United States by Oxford University Press lnc., New York
© D. G. Pettifor,
1995
All rights reserved. No parts of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, without the prior permission in writing of Oxford University Press. Within the UK, exceptions are allowed in respect of any fair dealing for the purpose of research or private study, or criticism or review, as permitted under the Copyright, Designs and Patents Act, 1988, or in the case of reprographic reproduction in accordance with the terms of licences issued by the Copyright Licensing Agency. Enquiries concerning reproduction outside those terms and in other countries should be sent to the Rights Department, Oxford University Press, at the address above. This book is sold subject to the condition that it shall not, by way of trade or otherwise, be lent, resold, hired out, or otherwise circulated without the publisher's prier consent in any form of binding or cover other than that in which it is published and without a similar condition including this condition being imposed on the subsequent purchaser. A catalogue record for this book is available from the British Library Library of Congress Cataloging in Publication Data Pettifor, D. G. (David G.), 1945Bonding and structure of molecules and solids / D.G. Pettifor. 1. Solid state physics. 2. Electronic structure. 3. Molecules. 4. Chemical bonds. 5. Composite materialsBonding. I. Title. 1995 541.2'2dc20 9532183 QC176.P443 ISBN 0 19 851787 4 (Hbk) ISBN 0 19 851786 6 (Pbk) Typeset by Integral Typesetting, Gt, Yarmouth, Norfolk Printed in Great Britain by Bookcraft (Bath) Ltd M idsomer Norton, Avon
Preface 'As simple as possible but not simpler' Albert Einstein Einstein's caveat is indeed an apt warning for those who wish to explain the structure of molecules and solids within a simple theory or set of rules. The difference in energy between competing structure types is very small, often being a mere hundredth or thousandth of the total cohesive energy. Simple valence bond arguments, for example, can rationalize the wellknown 8N rule for the structures of spvalent elements by assuming that single covalent bonds are formed between neighbouring atoms, thereby completing the stable octet shell of electrons about each atom. But how do we account for the many exceptions to the 8N rule such as group IV carbon and lead being most stable in the nonfourfold coordinated graphitic and cubic closepacked structure types respectively? The common assertion that the graphitic structure is stabilized by the formation of Sp2 hybrids on the carbon atoms is far too simplistic as the carbon atoms could equally well have formed Sp3 hybrids to stabilize the diamond structure instead. In practice, the most stable structure is determined by a delicate balance between opposing terms in the total binding energy. The ab initio prediction of which structure is the most stable by ·computing and comparing total energies appears at the outset to be a formidable task. The fundamental equation of quantum mechanics, the Schrodinger equation, can be solved exactly for the hydrogen atom. Its solution for the hydrogen molecule and for all other systems is a manybody problem. The wave function is now no longer dependent on the coordinates of a single electron but on the coordinates of all. the electrons. Unfortunately, the traditional HartreeFock approximation to solving the manybody Schrodinger equation was found to be insufficiently accurate for reliable structural predictions to be made for bulk materials, especially metals. A breakthrough occurred, however, in the mid1960s when Pierre Hohenberg, Walter Kohn, and Liu Sham proved that the total ground state energy of a manyelectron system is a functional of the density. This seemingly simple result, by focusing on the electron density rather than the manybody wave function, allowed them to derive an effective oneelectron Schrodinger equation which could be solved within the socalled local density approximation. Extensive computations during the past two decades have demonstrated the accuracy of local density functional theory in predicting the structural properties of a wide range of ionic, covalent, and metallic systems. This success of density functional theory allows the whole question of bonding and structure to be formulated within an effective oneelectron framework that is so beloved by chemists in their molecular orbital description of molecules and by physicists in their band theory description of solids. In this book I have tried to follow Einstein's dictum by simplifying the oneelectron problem to the barest
vi
Preface
essentials necessary for understanding observed trends in bonding and structure. In particular, the chemically intuitive tight binding approximation is shown to provide a unified treatment of the covalent bond in small molecules and extended solids, whereas the physically intuitive nearly free electron approximation is found to give a natural description of the metallic bond in spvalent metals. Emphasis is placed on recent theoretical developments that link structural stability to local topology or connectivity of the lattice through the moments of the electronic density of states. This moments approach creates a powerful bridge between the physicists' view of the global electronic structure in reciprocal space and the chemists' view of local bonding in real space. We will see that it leads to a fundamental understanding of the structural trends within the periodic table for the elements and within the AB structure map for binary compounds, experimental trends that are presented and discussed in the first chapter. This book is directed at finalyear undergraduates and firstyear postgraduates in physics, chemistry, and materials science who have already attended introductory courses on quantum mechanics and molecular orbital and/or band theory. I assume, therefore, that the reader is familiar with concepts such as the covalent bond, hybrid orbitals, and electronegativity. However, in order to understand the structural trends . that are observed amongst the elements and binary compounds, it is necessary not only to quantify these old concepts but also to introduce new concepts that extend our physical and chemical intuition. Both the quantification of old concepts and the development of new concepts requires the reader to take the plunge and to be swept along by the intemallogic and predictive power of the simple models presented in this book. Most of the illustrative examples in the text require no more mathematical ability than the solution of a quadratic equation. By working through these examples readers will gain insight and experience that allows the newly learned concepts to become part of their everyday intuition and vocabulary. This intuition may be further honed by problems at the end of the book. The plunge required for understanding the elegant secondorder perturbative treatment of the structure of spvalent metals is deeper and more bracing than that needed for solving a 2 x 2 secular equation, so that Chapter 6 could be omitted on a first reading of the book. This book is the product of many people's input and ideas. The importance of my past and present research students and postdocs is reflected in the credits to many figure captions. I should, however, like to mention in particular Nguyen Manh Due and Paul Lim who helped with a number of the illustrations. I should also like to acknowledge the very helpful comments of Sir Alan Cottrell, Volker Heine, and John Jefferson on the first draft of this book which had been magnificently typed by Beatrice May from a nearly illegible original text. And finally my wannest thanks to C. T. Liu who was amongst the first to appreciate the beauty and usefulness of the phenomenological structure maps, Masato Aoki who kept faith with the bond order potentials, Adrian Sutton who shares the dream of modelling materials across all the length scales, and Di Gold who provided love and support during the summer of '94 when this book was written.
Oxford June 1995
D.G.P.
Contents Note on the choice of units
1 . Experimental trends in bonding and structure 1.1. Introduction 1.2. Structures of the elements 1.3. Lattice types: the Pearson notation 1.4. Local coordination polyhedra: the Jensen notation 1.5. Bonding and structural trends within the elements 1.6. Bonding and structural trends within AB compounds 1.7. Structural trends within molecules References
2. Quantum mechanical concepts 2.1. Introd uction 2.2. Waveparticle duality 2.3. Heisenberg's uncertainty principle 2.4. The Schrodinger equation 2.5. The freeelectron gas 2.6. The free atoms 2.7. Quantum mechanical structural predictions References
3. Bonding of molecules 3.1. Introduction 3.2. Bond formation in svalent dimers 3.3. Electronegativity scales 3.4. Dissociation of the hydrogen dimer 3.5. (1, 7t, and () bonds 3.6. Bond formation in spvalent dimers 3.7. Hybrid orbitals References
4. Structure of molecules 4.1. Introduction 4.2. Structural stability: an illustrative example 4.3. The structural energy difference theorem
xi
,
1 1 5 6 10 12 17 19
20 20 20 26 29 31 35 45 49
50 50 50 57 60 66 68 74 76
77 77 77 81
viii
Contents 4.4. The structure of svalent molecules 4.5. Origin of structural trends: a moments theorem 4.6. The bond order 4.7. Linear versus bent triatomic molecules References
5. Bonding of spvalent metals 5.1. Introduction 5.2. Jellium: from small molecules to the bulk 5.3. General principles of band theory 5.4. The nearly free electron approximation 5.5. Pseudopotentials 5.6. The nature of the metallic bond in spvalent metals 5.7. Embedded atom potentials References
6. Structure of spvalent metals 6.1. Introduction 6.2. Screening: the ThomasFermi approximation 6.3. Screening: linear response theory 6.4. The reciprocal lattice representation 6.5. The realspace representation 6.6. Structural trends 6.7. HumeRothery electron phases References
85 91 96 100 106
107 107 108 111 118 121 127 131 135
137 137 137 139 145 150 156 166 171
7. Bonding of transition metals and semiconductors 7.1. Introduction 7.2. The tight binding approximation 7.3. Hybrid NFETB bands 7.4. The nature of the metallic bond in transition metals 7.5. The rectangular d band model of cohesion 7.6. The rectangular d band model of heats of formation 7.7. The saturated bond in semiconductors References
8. Structural trends within solids 8.1. 8.2. 8.3. 8.4.
Introduction Saturated versus unsaturated bonds Structural trends within the spvalent elements Interpretation in terms of moments
173 173 173 178 180 187 191 198 206
209 209 209 214 219
Contents
ix
8.5. Structural trends within the sdvalent elements 8.6. Anomalous structures due to magnetism 8.7. Structural trends within the pdbonded AB compounds 8.8. Bond order potentials References
223 226 232 239 240
Problems
242
Index
251
Note on the choice of units The energy and length scales that are appropriate at the atomic level are those set by the ionization potential and first Bohr radius of the hydrogen atom. In SI units the energy and radius of the nth Bohr stationary orbit are given by (1)
and (2) where m is the electronic mass, e is the magnitude of the electronic charge, 80 is the permittivity of free space, and Ji is Planck's constant divided by 27t. Substituting in the values m = 9.1096 x 10 3 1 kg, e = 1.6022 x 10 19 C, 4n8 0c 2 = 107 , C = 2.9979 X 108 mjs and Ii = 1.0546 X 10 34 Js, we have E = _ 2.1799 "
X
10
18
J
n2
(3)
and
a" = 5.2918 x 10 1 1n2 m
(4)
Therefore, the ground state of the hydrogen atom, which corresponds to n = 1, has an energy of 2.18 x 10 1 8 J and an orbital Bohr radius of 0.529 x 10 10 m or 0.529 A. The first value defines the Rydberg unit (Ry), the latter one the atomic unit (au). Thus, in atomic units we have
E" = _n 2 Ry
(5)
a" = n2 au
(6)
and where 1 Ry = 2.18 X 10 1 8 J = 13.6 eV and 1 au = 5.29 x 10 11 m = 0.529 A. It follows from (1), (2), (5), and (6) that Ji 2j (2m) = 1 and e2j(4n80 ) = 2 in atomic units. The total energy of the molecule or solid will usually be given in either Ryjatom or eVjatom. Conversion to other units may be achieved by using 1 mRyjatom = 1.32 kJjmol = 0.314 kcaljmol.
1 Experimental trends in bonding and structure
1.1. Introduction The crystal structures of the elements display wellknown trends within the periodic table. On a broad scale the closepacked structures that are characteristic of the metallic bond on the lefthand side give way to the more open structures of the covalent bond on the righthand side. On a finer scale, specific trends are observed such as the hcp + bee + hcp + fcc sequenee across the transitionmetal series or the 3fold coordinated graphitic + 4fold coordinated diamond + 12fold coordinated fcc sequence down group IV from C to Pb, The crystal structures of isostoichiometric binary compounds also display welldefined trends when the experimental data base is presented within a twodimensional structure map. In addition to structural domains reflecting closepacked metallic or open covalent bonding, ionic domains of stability appear, such as NaCI and CsCl regions amongst the alkali halides. This chapter presents the experimental structures of the elements and binary AB compounds and highlights the dominant structural trends. Each structure type will be characterized not only by one of the fourteen Bravais lattices, which defines the basic building block for global threedimensional periodicity, but also by the local coordination polyhedron about each nonequivalent site, which reflects the bonding type. Further, since our understanding of the nature of the chemical bond in solids must be compatible with a theory of the bonding and structure of molecules, the groundstate structural data base on trimers and elemental spvalent molecules with up to six atoms will be given.:
1.2. Structures of the elements Table 1.1 gives the structures of the elements at zero temperature and pressure. Each structure type is characterized by its common name (when assigned), its Pearson symbol (relating to the Bravais lattice and number of atoms in the cell), and its Jensen symbol (specifying the local coordination polyhedron about each nonequivalent site). We will discuss the Pearson and Jensen symbols later in the following two sections. We should note,
Table 1 .1 The gro und st ate str uctures of the elements H, 'drogen, nitrogen,oxygen.and Ihe halogens bi nd as d lrners Ina ' are Ihe." weakly held toge ther on the la ttices which are Indica ted by tILe Pearso n symbol. (Dat a from P. Villars and Da arns (1993»
u.c.
0 1 He LI R~li~l; lSlMlt h P2 hID
;12.'.1
is 1 ~ 1712~
Ne
.{5,wl: '
ti,
nnr
Ar
K
n.
n
nP2
hRI05 hP4
T2!,
,
15 N~
C
~,
..l:.. ,:; '3"
W'2
cP...... nw' ll)J!I!Ql. . ~ h1'2 cf4 cFB SI
AI
2
4
3
Ca
So
Ti
5 V
(,
Cr
7 Mn
8
9 Co
Fe
10
,. ij2''' TI~ Zn Ga
11
Ni
Cu
41"'"
I'
t
ltt!1~J!J
It
tr""  ,
G.
oCB
W' •
17
16
& \k hR2
.. it · : l;;:Vt ,.
I
hID
lk&_ uz= cN e12
flP2
14
R4l::i C:;:=1ENk, 1\'ep....
N~
I~
cF4
§.
Element C ommon n am e Pearson symbol [crs en symbol
13
12
~ 71 , The dashed curve gives the classical RayleighJeans law at temperature, T2 .
We will consider four key experiments which led to the unravelling of the classical world view, namely blackbody radiation, the photoelectric effect, Compton scattering, and electron diffraction. 1. Blackbody radiation: Figure 2.2 shows the frequency dependence of the
intensity of the radiation that is emitted from a black body at two different temperatures, T, and 1;, where 1; > Ti , We see that at high frequencies the emitted intensity, I, is much less than that predicted by the RayleighJeans law, namely (21)
where k B is the Boltzmann constant and A is a given constant This law follows from the fact that the number density of oscillating modes is proportional to ro 2 , and each mode has associated with it an average energy of kBT by the equipartition of energy, tkBT each for the average kinetic and potential energies of a classical oscillator, The deviation of theory from experiment implied the existence of some barrier to the emission (or absorption) of radiation at higher frequencies. To account for this, Planck assumed in 1900 that electromagnetic energy is not emitted or absorbed continuously but in discrete packets or quanta of energy E = hv
= hco
(22)
where h is Planck's constant and Ii = h/21t. A given oscillating mode of angular frequency, ro, then has associated with it a discrete spectrum of allowable energies E,. = nho: rather than the continuous spectrum of a classical simple harmonic oscillator. As illustrated schematically in Fig. 23 this leads to the highfrequency oscillators not being thermally activated at low temperatures. By Boltzmann statistics, the probability that the nth level
Waveparticle duality 23 E
E
r
11 I~T
fJ~
~J
Low frequency
Heat ba1h
fJ~~T
Fig. 2.3 Schematic illustration of how the quantization of the electromagnetic energy leads to the highfrequency modes being less easily thermally excited than the low frequency.
is excited depends exponentially on its energy, E,l' so that the average energy, (E), of a quantum oscillator of angular frequency, ro, is given by (2.3) which with En = nnro simplifies to (E)
= [(nro/kBT)/(e"tJ)/kBT 
1)]kBT.
(2.4)
At low frequencies (or high temperatures) when nro/kBT« 1. this reduces to the classical limit, (E) = kBT. since the prefactor in square brackets tends to unity using the Taylor expansion, exp x = 1 + x + .... At high frequencies (or low temperatures) when nrofkBT» I, this reduces to the exponential form, (E) = hco exp( nro/kBT), which accounts for the drop in intensity at high frequencies observed in Fig. 2.2. Fitting Planck's constant to the experimental curves gave n= 1.055 x 10 34 Is. This very small but non.. vanishing number has important consequences. The comforting image of red hot coals at l000 0K is associated with radiation being emitted at a wavelength of 7000 A, corresponding to nro/kBT = 1.8 eV/O.l eV = 18. In a classical world, therefore, this redhot radiation would be more than a million times more intense. At the same time the total energy in the ultraviolet spectrum would diverge catastrophically.
2. The photoelectric effect: Light incident on a clean metal surface ejects electrons with energies that depend only on the frequency but not on the intensity of the light. The intensity affects the number of electrons emitted.
24
Quantum mechanical concepts
This is impossible to understand within a wave description of light since an electromagnetic wave would exert a force on a stationary electron at the metallic surface that is proportional to the electric field and, hence, the electron would be emitted with a velocity dependent on the intensity of the incident light. In 1905 Einstein explained the photoelectric effect by regarding the incident radiation as a beam of particles comprising Planck's quanta with individual energies of hco. A single light quantum or photon would then kick out an electron from the surface with velocity, v, according to
!mv2 = hill  0
(2.5)
where m is the electronic mass and 0 is the surface work function. Equation (2.5) expresses the conservation of energy; the photon is annihilated during collision, giving up its energy, hill, to the electron, thus overcoming the work . function barrier, 0. The photon escapes into the vacuum with kinetic energy, jmv2 • Increasing the intensity of the light increases the number of incident photons. This leads to the emission of a greater number of electrons, but the velocities of these electrons remain unchanged as observed experimentally.
3. The Compton effect: A photon is characterized not only by its energy, E = hill but also by a momentum, p. The latter may be evaluated directly by using the relativistic expression for the energy of a particle in terms of its rest mass, m, and momentum, p, namely (2.6)
where c is the velocity of light. For a particle at rest, the famous identity, E = me", is recovered. For a photon with zero rest mass, E = pc. Hence, the momentum of a photon is given by p
E
hv
h
=  =  =  = hk, c c A
(2.7)
where we have used c = AV and k = 2n/A, or in vector form p
= hk.
(2.8)
In 1923, Compton measured the change in momentum of Xray photons during scattering by stationary electrons as illustrated schematically in Fig. 2.4. He found that the change in the wavelength of a photon, L\1, was related to the scattering angle, 9, through the very simple relation
L\A = 2A c sin 2 ~2'
(2.9)
where At was a constant. This result could not be understood within classical electromagnetic theory since Ac is then predicted to be a function of the incident wavelength rather than a universal constant. However, eqn (2.9) is
Waveparticle duality 25 Scattered
photon
incident photon
Recoiiing eiectron
Fig. 2.4 The scattering of a photon by a stationary electron in the Compton effect.
a direct consequence of applying energy and momentum conservation to the photonelectron scattering processing illustrated in Fig. 2.4. Using the relativistic expression eqn (2.6), the conservation of energy gives (210)
where Pl and P2 are the incident and scattered photon momenta, and m and Pe are the rest mass and scattered momentum of the electron respectively. The conservation of momentum, Pl = P2 + Pe, gives (2.11) Substituting eqn (2.11) into eqn (2.10), and taking CP2 to the lefthand side and squaring yields /
(2.12) Dividing by P1P2 and using P = hll, Compton's result, eqn (2.9), is recovered with lc = hlmc. The term lc is thus a constant as found experimentally, taking the value of 0.024 A, the socalled Compton wavelength.
4. Electron diffraction: In 1924, de Broglie postulated his principle of waveparticle duality. Just as radiation displays particlelike characteristics, so matter should display wavelike characteristics. It followed, therefore, from eqs (2.2) and (2.7) that a particle with energy, E, and momentum, Po has associated with it an angular frequency, OJ, and wave vector, k, which are given by (2.13) OJ = Eln and (2.14) k = pIn. The latter equation implies that a particle of momentum, P, has an associated wavelength, 1 = hlp, the de Broglie wavelength. This was verified a year
26
Quantum mechanical concepts
or so later by Davisson and Germer who demonstrated that electrons were diffracted from a nickel crystal as though they had the wavelength postulated by de Broglie.
2.3. Heisenberg's uncertainty principle How do we understand and describe this waveparticle duality? Clearly a plane wave, A exp[i(kx  rot)], has a welldefined angular frequency, ca (or energy), and wave vector, k (or momentum). But it is infinite in extent, with its intensity, IAI 2 , being uniform everywhere in space. In order to create a localized disturbance we must form a wave packet by superposing plane waves of different wavevectors. Mathematically this is written 'I'(x, t) =
_1_'fco
~
cP(k) ei1kx 
(O(k)t]
dk,
(2.15)
co
where the cP(k) are the amplitudes of the individual plane waves. The angular frequency, ro, is a function of the wave vector, k, through the dispersion relation, co = ro(k). At the time, t = 0, the wave packet, 'P(x,O), is given by
~ fco
'I'(x, 0) =
V 2n
cP(k) e ikx dk,
(2.16)
'I'(x, 0) e ikx dx,
(2.17)
 co
where by Fourier analysis 1 cP(k) =,r;:;:.. V 2n
fco  co
Let us consider the simple Gaussian wave packet, 'I'(x, 0)
= A e i kox e(Xxo)2/2 W2,
(2.18)
which from eqn (2.17) has the associated Gaussian amplitude cP(k) = AW eHko 
k)xo
e  W 2(k 
kO)2/2 •
(2.19)
We see from Fig. 2.5 that the Gaussian wave packet has its intensity, 1'1'1 2 , centred on Xo with a half width, W, whereas IcP(k)1 2 is centred on k o with a half width, I/W. Thus the wave packet, which is centred on X o with a spread Ax = + W, is a linear superposition of plane waves whose wave vectors are centred on ko with a spread, Ak = + I/W But from eqn (2.8), P = hk. Therefore, this wave packet can be thought of as representing a particle that is located approximately within Ax = W of X o with a momentum within Ap = h/W of Po = hk o. If we try to localize the wave packet by decreasing W, we increase the spread in momentum about Po. Similarly, if we try to characterize the particle with a definite momentum by decreasing I/W, we increase the uncertainty in position.
Heisenberg's uncertainty principle
27
Fig. 2.5 The relation between a Gaussian wave packet, '1', and its Fourier transformation, cPo The quantity, 1'1'12 , has a half width of W, where IcPI 2 has a half width of
W'.
This is a statement of Heisenberg's uncertainty principle, namely Ax x Ap ;  = h, 2n
(2.24)
which is consistent with Heisenberg's uncertainty principle. It is just not possiblein principleto measure position and momentum with absolute certainty. If we try to determine whether an electron is a wave. or a particle, then we find that an experiment which forces the electron to reveal its particle character (for example, one using a very short wavelength microscope) suppresses its wave character as Ap and hence Ak are large. Alternately, when an experiment focuses on the electron's wavelike behaviour, as in electron diffraction, Ak is small, but there is a correspondingly large uncertainty in the position of any given electron within the incident beam. What does the wave function, \f(r, r), actually represent? Consider the diffraction of an electron beam by two slits as illustrated in Fig. 2.7. Experimentally it is found that the diffraction pattern is not the result of the electrons travelling through slit 1 interfering with those from slit 2. The pattern persists even for the case when the intensity of the incident beam is so low that the particles travel singly through the system, being recorded as individual 'flashes' on the screen which build up to give the diffraction pattern observed. This led Born in 1926 to interpret. l\f(r, t)1 2 dr as the probability of finding the electron at some time, t, in the volume element dr = dx dy dz, which is located at r = (x, y, z). Since the probability of finding a given electron somewhere in space is unity, the wave function of
The Schrodinger equation
29
2
r 1
Electron beam
Slits
SCreen
Fig. 2.7 Diffraction of an electron beam by two slits.
a single electron 'must satisfy the normalization condition
J
1'I'(r,
t)1 2 dr =
1.
(2.25)
all space
2.4. The Schrodinger equation In classical mechanics, Newton's laws of motion determine the path or time evolution of a particle of mass, m. In quantum mechanics what is the corresponding equation that governs the time evolution of the wave function, 'I'(r, t)? Obviously this equation cannot be obtained from classical physics. However, it can be derived using a plausibility argument that is centred on the principle of waveparticle duality. Consider first the case of a free particle travelling in one dimension on which no forces act, that is, it moves in a region of constant potential, V. Then by the conservation of energy
E = p2 / 2m + V.
(2.26)
But by de Broglie's principle of waveparticle duality, this free particle has associated with it a wave vector, k = pIn, and angular frequency, ro = Eln (cf eqs (2.13) and (2.14)), which substituting into the above equation gives
hca =
n k / 2m + V. 2 2
(2.27)
However, this dispersion relation is just that obtained by solving the partial differential equation a'l'(x, t) _ iii    at
2 2'1'(x, n a t) r.rm( ) +" x. r).
2m
ax':
T
(2.28)
This can be seen directly by substituting into it the plane wave solution,
'I'(x, t) = A ei(btof).
(2.29)
30
Quantum mechanical concepts
We now make the ansatz that the form of this partial differential equation does not change if V = V(x, t) rather than a constant. Generalizing eqn (2.28) to three dimensions, we find the timedependent Schrodinger equation, h2
. 8'1'
2
Ih  =   V 'I' 8t 2m
+ V'P
(2.30)
'
where V2
82 =_2 +_ 8x 8y 2 82
82
+ _2. 8z
We note the very important property that this equation is linear so that if '1'1 and '1'2 are solutions, so also is A1'P1 + A 2'P 2 , generalizing the linear superposition of plane waves we saw earlier. The timedependent Schrodinger equation may be solved by the method of separation of variables if the potential does not depend explicitly on time, that is, V = V(r). Writing 'P(r, t) = t/J(r)T(t), substituting it into eqn (2.30) and dividing by t/J(r)T(t) we have
in. ~ dT =.!. [~ V2t/J + V"'] T dt t/J 2m
= ex,
(2.31)
where ex is the usual separation constant. Thus
11t) = e iat/It
(2.32)
represents an oscillatory function of angular frequency, ex/h. But by de Broglie's equation (2.13), OJ = E/h, so that ex = E. Hence 'PE(r, t) = t/JE(r) e iEt/It,
(2.33)
where from eqn (2.31) the spatially dependent term, t/JE(r), is an eigenfunction of the timeindependent Schrodinger equation h 2 2t/JE(r)  V
2m
+
Vt/JE(r) = E"'E(r).
(2.34)
A system is said to be in a stationary state of energy, E, when it is represented by a wave of type eqn (2.33), since then the probability density is independent of time as 1'P:(r, t)'PE(r, t)l = l"'E(r)1 2 • We should note that the Schrodinger equation is nonrelativistic since we derived it from the nonrelativistic expression for the energy eqn (2.26). The Dirac equation is the relativistic analogue that is based On the relativistic expression for the energy, namely eqn (2.6). It led directly to the novel concept of electron spin. Since the valence electrons, which control the cohesive and structural properties of materials, usually travel with velocity v« C, they are adequately described by the Schrodinger equation. For the heavier elements, such as the lanthanides and actinides, relativistic effects can be included perturbatively when necessary. Photons, the quanta of the
The freeelectron gas 31 electromagnetic field, travel at the speed of light and have zero rest mass, so they require the separate treatment of quantum electrodynamics.
2.5. The freeelectron gas The spvalent metals such as sodium, magnesium and aluminium constitute the simplest form of condensed matter. They are archetypal of the textbook metallic bond in which the outer shell of electrons form a gas of free particles that are only very weakly perturbed by the underlying ionic lattice. The classical freeelectron gas model of Drude accounted very well for the electrical and thermal conductivities of metals, linking their ratio in the very simple form of the WiedemannFranz law. However, we shall now see that a proper quantum mechanical treatment is required in order to explain not only the binding properties of a freeelectron gas at zero temperature but also the observed linear temperature dependence of its heat capacity. According to classical mechanics the heat capacity should be temperatureindependent, taking the constant value of !k B per free particle. The Schrodinger equation for a freeelectron gas takes the form
_~ ((}22 + (}2 + ~)r/J(r) = 2m iJx
iJ y 2
iJ z2
Er/J(r).
(235)
If the electrons are confined within a box of side L, then the normalized eigenfunctions are the plane waves (2.36) which can be seen by writing k·r as k~x + kyy + k:zz and substituting into eqn (2.35). The corresponding eigenvalue is given by h2 2 E= ~ (k 2m~
+ ky2 + k:z2 ) =
h2 2m
~ k2 •
(2.37)
For a free electron this energy is purely kinetic, so that E = p2/2m. Hence p = hk = hl); as we have already found experimentally for free particles, namely eqs (2.8) and (2.14). The wavelength, .A., of the plane wave is constrained by the boundary conditions at the surface of the box. Imposing periodic boundary conditions on the box, which corresponds physically in one dimension to joining both ends of a metallic wire of length, L, into a closed ring, we have that r/J(x +:L, y, z) = r/J(x, y, z), r/J(x, y + L, z) = r/J(x, y, z), and I/!(x, y, z + L) = r/J(x, y, z). Hence, from eqn (2.36), k
=2n (n~, ny, n:z), L
(2.38)
32
Quantum mechanical concepts ••••••••
•••• ••
'.0
•••••••
·.0
••••••••••
•••••
II
•••••••••
0
••••••••••••••••••••••••••••
•••••••••
0_
,
••••••••••••••••••••
0"
•••••••••••••
•••••
•
••
0
••••••••
eo· •• ••• •• 
0".· I
••••••
•••••••••
::::::::::::::::::::::::::::::; ::::::::::; :;::::; ::;:::~: ::: '.0
••••••••• 0
II
•••••••••••• 0
_
••••••••
'"
•••••••••
0
eo
•••••
O
,
••
0
........................................................... ••••••
••••
•••••••••
•••••
•••••••
•••••••
••••••
•••••••
••••
0
•••
••••••••
•••••••
0
••
•
•
0
••
••• 0
·0
•• ,
••••••••••
•••••••••••••••••
Fermi'S'p"here'::::::: ::;: ;:::::::::::::::::'::::::::::::: •• _
..... ...,. ............. . ·..... .......... ............... . ·· ··· ....... .......... ••••
0
••
,
"0 •••••••••••••••••••••••
•••••••••••••••••••••••••••••••••••
'
,
,
..
~
......

:
.. .. .. .. . ... .
Fig. 2.8 The fine mesh of allowed kvalues. At zero temperature only the states k within the Fermi sphere are occupied.
(b) n(E}
(a)
E
o
EF
E
Fig. 2.9 (a) The free electron dispersion, E(k). (b) The density of states, neE).
where nx • ny • and n, are integers. Thus. the allowed values of the wave vector. k, are discrete and fall on a fine mesh as illustrated in Fig. 2.8. Following Pauli's exclusion principle. each state corresponding to a given k can contain at most two electrons of opposite spin. Therefore. at the absolute zero of temperature all the states. k, will be occupied within a sphere of radius. k F • the socalled Fermi sphere because these correspond to the states of lowest energy. as can be seen from Fig. 2.9(a). The magnitude of the Fermi wave vector. k F • may be related to the total number of valence electrons N by (2.39) !nk~2(LI2n)3 = N. since it follows from eqn (2.38) that unit volume of kspace contains (L/2n)3
The freeelectron gas 33
states capable of holding two electrons each. Thus. (2.40)
where p is the density of the gas of free electrons. p = N/ L 3. and rs is the radius of the sphere containing on average one electron. that is (2.41)
The corresponding Fermi energy. EF • equals 1i2k~/2m. This takes the values 3.2, 7.1. and 11.6 eV at the electronic densities. of sodium. magnesium. and aluminium. which are close to the experimental values for the occupied bandwidths. namely 2.8. 7.6. and 11.8 eV respectively. The freeelectron density of states n(E) may be obtained directly from eqn (2.39) by writing it in the form (2.42) where N(E) is the total number of states of both spins available with energies less than E. Differentiating with respect to energy gives the density of states (2.43)
which is illustrated in Fig. 2.9(b). We can now see why the experimental electronic heat capacity did not obey the classical result of !kB per electron. Following Pauli's exclusion principle, the electrons can be excited into only the unoccupied states above the Fermi energy. Therefore. only those electrons within approximately k B T of E F will have enough thermal energy to be excited. Since these constitute about a fraction kBT/E F of the total number of electrons we expect the classical heat capacity of !kBN to be reduced to the approximate value (2.44)
where the Fermi temperature is defined by E F . = kBTF • (If the calculation is performed exactly. using the squareroot dependence of the density of states. then the prefactor changes by the amount. n 2 /3.) For the simple metals magnesium and aluminium. the Fermi temperature is of the order of 100.000 K. so that the electronic heat capacity at room temperature is dramatically reduced compared to the classical prediction for a freeelectron gas. The above model of an spvalent metal as a gas of free electrons would exhibit no bonding because the only contribution to the energy is the repulsive kinetic energy. It takes an average value per electron, which is given
by
(2.45)
34
Quantum mechanical concepts
Using eqn (2.40) this may be written explicitly in terms of rs as
Uke = 2.210/r;,
(2.46)
where atomic units have been used so that length is measured in units of the first Bohr radius of hydrogen, namely 1 au = 0.529 A, with energy in units of the ionization potential of hydrogen, namely 1 Ry = 13.6 eV. We have so far made two implicit assumptions. The first of these is that the gas of electrons is not scattered by the underlying ionic lattice. This can be understood by imagining that the ions are smeared out into a uniform positive background The second assumption is that the electrons move independently of each other, so that each electron feels the average repulsive electrostatic field from all the other electrons. This field would be completely cancelled by the attractive electrostatic potential from the smearedout ionic background. Thus, we are treating our spvalent metal as a metallic jelly or jellium within the independent particle approximation. In practice, however, the motion of the particles is correlated: parallel spin electrons keep apart from each other following Pauli's exclusion principle, and antiparallel spin electrons keep apart to lower their mutual coulomb repulsion. For interacting electrons the former leads to a lowering in the energy by an amount called the exchange energy, the latter by an amount called the correlation energy. For a homogeneous electron gas, the average exchangecorrelation energy per electron is given in atomic units by Uxc
= 0.916/rs

(0.115  0.0313ln rs ) ,
(2.47)
where the first and second terms represent the exchange and correlation energies respectively. In order to understand this lowering in energy, imagine each electron accompanied by its own mutual exclusion zone or exchangecorrelation hole, as illustrated schematically in Fig. 2.10. Each electron now sees an additional attractive potential from the surrounding positive jellium background, which is not screened by electrons. Since the potential at the centre of a sphere of uniform charge varies inversely with the sphere radius, we expect the electron to feel an additional attractive potential proportional to l/rs • This is, indeed, the dominant term in the expression for the exchangecorrelation energy, namely eqn (2.47). The latter has been obtained by using the correct form of the exchangecorrelation hole, which has a diffuse boundary rather than the sharp boundary assumed in Fig. 2.10. The resultant binding energy of the freeelectron gas,
(2.48) is now attractive, as shown in Fig. 2.11. The maximum cohesion corresponds to a value of 0.16 Ry or 2.2 eV per electron at an effective electronic radius of 4.23 au or 2.2 A. This is not a bad description of the simple metal sodium, for at equilibrium, it has an experimental cohesive energy of 1.1 eV and an
The free atoms
35
Fig. 2.10 Schematic illustration of the mutual exclusion zone or exchangecorrelation hole about a given electron within a freeelectron gas. The hole has a radius, 's' corresponding to exactly one electron being excluded, thereby revealing one positive charge of underlying jellium background. The electron plus its positive hole move together through the gas of other electrons as though they are a neutral entity or quasiparticle.
Ueg
(Ry/e1ectron)
4.2
Fig. 2.11 The binding energy of a freeelectron gas as a function of 's' effective electronic radius of 4.0 au. However, although the other simple metals also have approximately 1 eV per valence electron of binding energy, they show marked variation in their equilibrium atomic volumes and corresponding values of This reflects the discrete size of the ions which has been lost in the jellium model. The important influence of the ion cores on the bonding and structure of the simple metals will be considered in detail in Chapters 5 and 6 respectively.
'S'
2.6. The free atoms The freeelectron gas model is agood starting point for the spvalent metals where the loosely bound valence electrons are stripped off from their ion cores as the atoms are brought together to form the solid. However, bonding in the majority of elements and compounds takes place through saturated
36
Quantum mechanical concepts
or unsaturated covalent bonds that form between relatively tightly bound valence orbitals describing, for example, the Sp3 hybrids in semiconductors or the d electrons in transition metals. The constituent free atoms then provide. the most natural starting point for characterizing the bonding in these tightly bound systems. The oneelectron Schrodinger equation for an isolated free atom takes the form ;'2
  V2 r/J(r) + V{r) r/J(r) = Er/J(r),
2m
(2.49)
where V(r) is an effective potential representing the interaction with the nucleus and the other electrons present (cf eqn (2.61». Since the potential, V(r), is spherically symmetric the solution takes the separable form
(2.50) where r, (), and ¢ are spherical polar coordinates and YT«(), ¢) are spherical harmonics. Just as the eigenfunctions for an electron in a cubic threedimensional box are characterized by the three quantum numbers, n,x, ny, and nz , that enter through the boundary conditions (cf eqn (2.38», so the eigenfunctions of an electron in a spherically symmetric threedimensional atom are characterized by threequanturn numbers, namely n, the principal quantum number, with n = 1,2,3,. "
I, the orbital quantum number, with 1 = 0, 1, ... , n  1 m, the magnetic quantum number, with m
= 0, + 1, ... , + I.
The principal quantum number, n, determines the energy of the hydrogen atom. The orbital quantum number, I, gives the magnitude of the orbital angular momentum, namely JI(I + 1);'. Electrons with orbital quantum numbers, 1 = 0, 1, 2, and 3 are referred to as s, p, d, and f respectively, after the old terminology of sharp, principal, diffuse, and fine spectroscopic lines. The magnetic quantum number, m, specifies the component of the angular momentum in a given direction, taking the (21 + 1) values, m1i, with Iml ~ 1. Because the energy of an electron cannot depend on the direction of its angular momentum in a spherically symmetric potential, these (21 + 1) states have the same energy and are said to be degenerate. The magnetic quantum number, m, is so called because this degeneracy is lifted in a magnetic field, which fixes a unique direction In addition, a relativistic treatment of the electron introduces a fourth quantum number, the spin, Ins, with m, = +t. This is because every electron has associated with it a magnetic moment which it quantized in one of two possible orientations: parallel with or opposite to an applied magnetic field.
The free atoms
37
The magnitude of the magnetic moment is given by
JI = 2.00~s(s + 1)JIB'
(2.51)
where s = Imsl =! and JIB = en/2m (the Bohr magneton). Each eigenstate nlm may, therefore, be doubly occupied by an up (ms = +t) and down (ms =  t) spin electron. Consequently any given Istate of a free atom will be 2(21 + 1) fold degenerate so that an sshell can hold 2 electrons, a pshell 6 electrons, a dshelll0 electrons, and an fshell14 electrons. This electronic shell structure, of course, underpins the periodic table. The Schrodinger equation can be solved exactly for the case of the hydrogen atom (see, for example, Chapter 12 of Gasiorowicz (1974». If distances are measured in atomic units, then the first few radial functions take the form (2.52)
R 2s() r 
1 (1 j2
1.) r/2 2r e ,
(2.53)
and
1 r/2 R 2p() r = ;;:;; r e . y24
(2.54)
They are given by the dashed line curves in Fig. 2.12. A conceptually useful quantity is the probability of finding the electron at some distance, r, from the nucleus (in any direction) which is determined by the radial probability density, ~I(r) = r 2R;I(r). We see from the full line curves in Fig. 2.12 that there is a maximum probability of locating the electron at the first Bohr radius, a b for the Is state and at the second Bohr radius, a 2 , for the 2p state. The average or expectation value of the radial distance, r, is given by _ (2.55) so that '15 = 1.5a b ~s = 1.5a 2 , and '2p = 1.25a 2 • Therefore, the 2s orbital is more extended or diffuse than the corresponding 2p orbital as is evident from Fig. 2.12. This is due to the fact that all solutions of the Schrodinger equation must be orthogonal to one another, that is, if "'111m and "'1I'I'm' are any two solutions and is the complex conjugate of "', then
"'*
f.p:,•.p
.'1'.'
dr = 0,
(2.56)
If the states have different angular momentum character then the angular integration over the spherical harmonics guarantees orthogonality. But if the states have the same angular momentum character then the orthogonality
38
Quantum mechanical concepts Bohrradius.an
a1
t
~
~
0.2
0.2;J....£~
0.5 P1S
0.25
o
5
10
!(au.)
Fig. 2.12 The radial function. R nl (dashed lines) and the probability density. Pnl (solid lines) as a function of , for the 1s. 2s and 2p states of hydrogen.
constraint implies that
fa'" R.,(r)R._,(r)r
2
dr = O.
(2.57)
Thus, for the 2s radial wave function to be orthogonal to the Is radial function, it must change sign, thereby accounting for the node at r = 2 au in Fig. 2.12. Similarly, the 3s radial function must be orthogonal to the 2s and, therefore, has two nodes, the 4s has three nodes, etc. Just as the energetically lowest Is state has no nodes, so the 2p, 3d, and 4f states are nodeless, since they correspond to the states of lowest energy for a given 1. The concept of the size of an atom is not well defined within quantum mechanics. An atom has no sharp boundary; the probability of finding an electron decreases exponentially with distance from the atom's centre. Nevertheless, a useful measure of the size of the core is provided by the position of the outer node of the valence electron's radial function, since we have seen that the node arises from the constraint that the valence state
The free atoms
39
0,,, """'' ..... ... ......... .. .....•.=.: 6p =:.:..:::••  .• :::.:.::~
'.._
··
~_6s
....~..:.:.,..........
....~

....__·············45
r
oct
5
"".~...
.·.......5
....:.::......
p
········4p ........ ....
c:
25
10
IA IIA
ns mB mBW~BEIB
li Be B C Ho Hg Al Si K Cll ••• Zn Gil Ge Rb Sr. Cd In Sn Cs Bll" Hg Tl Pb
N P As Sb BI
F Ne S CI A Se Br ICr Te I Xe Po At Rn Q
_~1
2p
IA DA
BB
ma:mB'SlB~BmB
Fig. 2.13 The negative of the inverse sand p pseudopotential radii of Zunger (1980).
must be orthogonal to the more tightly bound core states. This reflects Pauli's exclusion principle, which states that no two electrons may occupy the same quantum state. A notunrelated measure of size has been adopted by Zunger (1980), who determined Idependent radii, R" directly from first principles pseudopotentials (cf Chapter 5). Figure 2.13 shows his values of _R;l and _R;l for the spbonded elements. We see that the inverse Zunger radii of the free atoms vary linearly across the periodic table unlike the nearestneighbour distance in diatomic molecules or the equilibrium atomic volume in bulk systems, which varies parabolically due to the bonding between neighbouring atoms (cf Chapters 3 and 7). As expected, the sand p radii contract across a period as the nuclear charge increases, and they expand down a column as additional full orbital shells are pulled into the core region. One notable exception, however, is given by the crossing of the valence 3s and 4s radii, and also the valence 3p and 4p radii, at group BIB. This corresponds to Ga having a smaller core than AIdue to the fact that the former sits at the end of the 3d transition metal series across which the size of the core has shrunk due to the increase in the nuclear charge. It is not surprising, therefore, that the string through the periodic table in Fig. 1.8 reverses the order of Al and Ga. In addition, we see that the sizes of the secondrow elements B, C, N, and 0 are a lot smaller than those .of the other elements in their respective groups, which is again reflected by the string in Fig. 1.8 not linking B, C, N, and 0 to the isovalent elements in their respective groups.
40
Quantum mechanical concepts
Table 2.1 Atomic and ionic radii across the lanthanides. (The former corresponds to a bulk coordination of 12, the latter to an M 3 + ion with coordination of 6.) (After Douglas et al. (1983).) 0
Radii (A)
La
Ce
Pr
Nd
Pm
Sm
Eu
Gd
Atomic Ionic
1.877 1.172
1.82 1.15
1.828 1.130
1.821 1.123
1.11
1.802 1.098
2.042 1.087
1.802 1.078
Radii (A)
Tb
Dy
Ho
Er
Tm
Vb
Lu
Atomic Ionic
1.782 1.063
1.773 1.052
1.766 1.041
1.757 , .030
1.746 1.020
1.940 1.008
1.734 1.001
0
Another important example of the influence of core contraction on structural properties is provided by the lanthanides. Table 2.1 gives both their atomic and ionic radii, the former for a bulk coordination of 12, the latter for the triply charged positive ion with a coordination of 6. Firstly, we note that Eu and Yb have much larger atomic volumes than the other lanthanides. This is because they behave as divalent elements in the bulk metal due to the extra stability that arises from a halffull (f") or completely full (fI4) shell. We see in Fig. 1.8 that they are separated out and grouped after the divalent alkaline earths. Secondly, we note the marked contraction across the series, lutetium's atomic and ionic radii being 8% and 15% smaller than lanthanum's. This socalled lanthanide contraction causes the subsequent Sd valent element Hf to have a 1% smaller atomic radius than 4d isovalent Zr. This is reflected by the ordering of the string through .group IV in Fig. 1.8. The 4d trivalent element, Y, has an atomic radius that is about midway between that of La and Lu. It is, therefore, not surprising that it is found to be slotted in between Tb and Dy in Fig. 1.8. What is surprising, however, is that the string runs from Lu to La across the series rather than from La to Lu. The latter would have been in the direction of decreasing core size, which is reflected elsewhere in the periodic table as the string moves from left to right. In the last chapter we will see that this apparently anomalous ordering is due to the change in the relative population of the 5d and 6s valence states across the trivalent lanthanides. . The angular character of the orbitals, which is central to directional bonding, is determined by the appropriate spherical harmonic in eqn (2.50). For m = 0 the first few sphericalharmonics are. given by .
o 1 Yo =   ,
J4;r
Y o1 =
j{;'3 cos (), 4n
(2.58)
(2.59)
The free atoms 41
z
s y
Fig. 2.14 The angular dependence of the s. Pz and d 3z 2 _ r2 orbitals. The origin of the Cartesian axes passes through the centre of each individual orbital in the directions drawn.
and
y~ =
J
5 (3 cos! /I  1).
16n
(2.60)
These are plotted in the yz plane in Fig. 2.14. We see that the s state is spherically symmetric, taking the same positive value in all directions. The p state (1 = 1, m = 0), on the other hand, has a positive lobe pointing out along the positive z direction, but a negative lobe pointing out along the negative z direction. Note that these two lobes are spherical, since the plot, r = [cos 01, corresponds to x 2 + y2 + (z + t)2 = i using the relation z = r cos O. This state is not surprisingly referred to as a pz orbital. The d state (1 = 2, m = 0) has positive lobes along the z axis with a negative lobe in the equatorial xy plane. This state is referred to as a d 3z2 _;2 orbital, or simply dz2 . We will see later that the signs of the lobes are very important when considering the overlap of orbitals during bonding. It is clear from Fig. 2.14 that the sign of the sand d states are unchanged on inversion about the origin (i.e. they are even or gerade) whereas the p state changes sign (i.e. it is odd or ungerade). Figure 2.15 shows the corresponding probability clouds /Yj(O, cf»/2 that give the angular dependence of the probability density 1"'"I",(r)12. Comparing with the previous figure we see that the s state remains spherical whereas the lobes of the pz state are distorted from sphericity along the z .axis, reflecting the change from cos 0 to cos! O. Since we often deal with .atoms in a cubic environment, it is customary to form p% and P, orbitals by taking linear combinations of the two remaining 1 = 1 states corresponding to m = + 1. They are illustrated in Fig. 2.15(b). Note that a full p shell has spherical symmetry since x~ + y2 + Z2 = r 2 • The probability clouds of the five d orbitals corresponding to 1 = 2 are shown in Fig. 2.15(c). As might
42
Quantum mechanical concepts z
s x
1=0
p
m=O
z
z
z
Pz
Px
Py
1=1 d
m=±1 z
z
z x
m=±1
z
z x
/=2
x
m=±2
Fig. 2.15 The probability clouds corresponding to s, p and d orbitals are shown in (a), (b), and (c) respectively.
be expected from Fig. 2.15, we will find in the following chapters that the structure of molecules and solids is very sensitive to the angular character of the valence orbitals. The energy levels of the hydrogen atom are determined solely by the principal quantum number, n, through E n ·=  n2 Rydbergs. In general, however, states with the same principal quantum number n, but different orbital quantum numbers, 1, have their degeneracy lifted because the presence of more than one electron outside the nucleus leads to the potential V(r) no longer showing the simple inverse distancedependence of the hydrogenic case. This is illustrated in Fig. 2.16 where it is clear, for example, that
The free atoms 43
>cu
IA nA Li B. H1I 1'111  
30 IA nA
name I9a1la~e1ZlIa B
(
H
AI Si P J( (0 .•.•• In Go G. As Rb Sr  .  (d In Sn Sb (s Bo'._Hg TI Pb Bi
2p
0
F Ht
S Se T. P
(I A Br Kr 1 X, At Rn
Fig. 2.16 Thevalences and p energy levels (after Herman and Skillman (1963».
the valence 2s level of the secondrow elements B to Ne lies well below that of the corresponding valence 2p level. These atomic energy levels of the valence electrons were taken from the tables compiled by Herman and Skillman (1963) who solved the Schrodinger equation numerically for all elements in the periodic table. Figure 2.16 illustrates several important features to which we will be returning throughout this book. 1. The valence energy levels vary linearly across a given period just like the inverse radii in Fig. 213. As the nuclear charge Ze increases, the electrons are bound more tightly to the nucleus. However, rather than varying as Z2, which would be the result for the energy levels of a hydrogenic ion of charge Ze, the presence of the other valence electrons induces the linear behaviour observed. 2. The valence s "and p energy levels become less strongly bound as one moves down a given group, and the value of the principal quantum number increases. This is to be expected from the 1/n2 dependence ofthe hydrogenic energy levels. But there is an exception to this rule: the 4s valence level has come down and crosses below the 3s valence level to the left of group VB. This is a direct consequence of the presence of the occupied 3d shell whose electrons do not completely screen the core from the valence 4s electrons, which therefore feel a more attractive potential than their 3s counterparts in the preceding row. This reversal in the expected ordering of the valence s energy levels is reflected in the ordering of the string between
44
Quantum mechanical concepts Or.....,....r.r.rrt
> 10 QJ
QJ
> QJ
u
E
o
B),
(3.66)
where 4>A and 4>B are the hybrid orbitals ,I,.
'¥A
= fi _1_ [1 + A /(1 + ..1 2 )1/2]1/2.,; + _1_[1  A /(1 + ..1 2 )1/2]1/2. ,; sp sp ¥'As fi sp sp ¥'A~ (3.67)
4>0 = ~ [1 + Asp/ (1 + A;p)I/2]1/2t/JBs y2
~ [1 
y2
Asp/ (1 + A;p)I/2]1/2t/J~.
.
(3.68) These are shown in Fig. 3.15 for the case of maximum mixing or hybridization that occurs for Asp = 0, when E, = E p , so that the two hybrids are given by (1/ fi)(t/Js + t/Jz)' It follows from eqs (3.67) and (3.68) that the fraction of s character in the hybrid is given by t[1 + Asp/ (1 + A;p)1/2] which, therefore, varies from 0.5 for Asp = 0 to 1 for Asp = 00. We see from eqn (3.66) that the bonding combination of the two sp hybrids (l/fi)(t/Js + t/Jz) and (l/fi)(t/Js  t/Jz) does not give the correct solution in general due to the nonvanishing sp splitting. (This splitting can be large, cf C 2 and Si2 in Fig. 3.13.) Although these are the most directed hybrids that lead to the largest overlap and bond integral (for the particular choice [sse] = ppC1), a penalty has to be paid because electrons must be promoted from the lowlying s state into the highlying p state that is mixed in. The
Hybrid orbitals 75
Fig. 3.15 Formation of the two sp hybrids, (1/)2)("'5 + "'z)' (After Huheey et el. (1993).)
eigenfunction optimizes the energy gain from overlap against the energy loss from promotion. In fact, we can split the energy of the most bonding state into two parts as
J
E;, = 21 (tPA + tPB)H(tPA A
1 + cPB) dr = !(H AA + H BB ) + HAB
(3.69)
where HAA , HBB , and HAB are the Hamiltonian matrix elements with respect to the hybrid orbitals tPA and tPB' Substituting eqs (3.67) and (3.68) into (3.66) and neglecting the overlap contributions we find
and
HAl) = [1
+ (I + ~p)112}hl,
(3.71)
where we have used eqn (3.58), namely ppa = spa =  sse =  h. Thus, adding eqs (3.70) and (3.71) we recover Ea ,
= E  Ihl  (1 + ~;p)1/2Ihl
(3.72)
as expected from eqn (3.59). This energy is lower than the energy of E  21hl that would have resulted from using the sp hybrids, (l/J2)(t/Js + t/Jz)' Although the bond integrallHABI is decreased from 21hl to {I
+ 1/(1 + ~;p)1/2]lhl,
the cost in promoting electrons into p states is reduced by the larger amount
76
Bonding of molecules
[A;p/(1 + A;p)1/2]lhl. This leads to the total energy being lowered by the amount [(1 + A;p)1/2  l]lhl which is observed in eqn (3.72). It is commonly asserted that hybrid orbitals are responsible for the groundstate structures that are observed. For example, carbon takes the graphitic structure due to Sp2 hybrids, whereas silicon takes the diamond structure due to Sp3 hybrids. However, as has been shown by the above discussion, the actual hybrid chosen is a delicate balance between two opposing factorsthe one trying to maximize the bond overlap with neighbouring atoms, the other trying to minimize the promotion energy. Structural prediction requires a careful treatment of the different competing terms in the total energy. We address this area for the case of molecules in the next chapter.
References Cotton, F. A. and Wilkinson, G. (1980). Basic inorganic chemistry. Wiley, New York. Gunnarsson, 0., Harris, J., and Jones, R. O. (1977). The Journal of Chemical Physics
67,3970. Gunnarsson, O. and Lundquist, B. I. (1976). Physical Review B13, 4274. Harris, 1. (1984). The electronic structure of complex systems (00. P. Phariseau and W. M. Temmerman), page 141. Plenum Press, New York. Huheey,1. E., Keiter, E. A., and Keiter, R. L. (1993). Inorganic chemistry: principles of structure and reactivity. Harper Collins, New York. Mulliken, R. S. (1934). Journal of Chemical Physics 2, 782. Pauling, L. (1960). The nature of the chemical bond. Cornell University, Ithaca, New York State. Phillips,1. C. and Van Vechten, J. A. (1969). Physical Review Letters 22, 705. Skinner, A. J. and Pettifor, D. G. (1991). Journal of Physics: Condensed Matter 3,
2029.
4 Structure of molecules 4.1. Introduction Molecules show a wide variety of structure, the number of variants increasing dramatically with number of atoms in the molecule, Thus, whereas the dimer displays only one structure type, the trimer can be either linear like CO2 or bent like H 2 0 . Molecules with four atoms, on the other hand, can take the onedimensional linear chain structures like H 4, the twodimensional square ring structure like S4 or the rhombic closepacked planar structure like Si4,· the threedimensional tetrahedral structure like P4' or numerous other distorted structural variants. The fiveatom molecule, as we have already seen in Fig. 1.15, chooses the closepacked plane as its ground state structure for Naj, the trigonal bipyramid for M~ and Sis, the regular pyramid for AJ s, and the envelope structure for S, respectively. The sixatom molecule can choose between the onedimensional linear chain, the twodimensional hexagonal ring or closepacked plane, the threedimensional pentagonal pyramid, trigonal tripyramid, trigonal prism, or octahedronto name but a few! The energy difference between these competing structure types is usually very small, often being of the order of 1% of the binding energy or less. Hence, the reliable prediction of the groundstate structure of a particular molecule requires selfconsistent quantum mechanical calculations of high precision that expend large amounts of computer time. In this chapter we will instead extend the simple ideas of dimeric bonding to larger molecules with up to six atoms, in order to study the structural trends that are observed as a function of the electron count or total number of valence electrons. We will see that the oscillatory trends in structural stability can be linked directly to the topology of the molecule through a very important moments theorem, which was first introduced into this area by Ducastelle and CyrotLackmann in 1971.
4.2. Structural stability: an illustrative example The relative stability of different structures is determined by a delicate balance between competing contributions to the total energy. This is illustrated by the following example in which we examine the stability of fouratom molecules with respect to the ideal linear chain, square, rhombus
78
Structure of molecules 1
4
1
3
3
3
Fig. 4.1 The linear chain, square, rhombus, and tetrahedron geometries of fouratom molecules.
or tetrahedron as shown in Fig. 4.1. We will simplify the problem by assuming that the energetics is describable by interatomic pair potentials so that the binding energy of the molecule may be written
u = ! L' ~Rij)'
(4.1)
i.j
where (Rij) is a central pair potential that is only dependent on the internuclear separation, R jj , between atoms i and j in the molecule. Following our discussion of the dimeric bond centred on eqn (3.46), we will divide up the pair potential into a repulsive and a bonding contribution, namely (4.2) (The constant shift, Va)' in eqn (3.46) need not concern us here since it is the relative stability of the different structures that we wish to predict in this chapter.) Around the equilibrium bond length, R o, the two contributions in eqn (4.2) may be related by
rcp(R) = AIboniR)I",
(4.3)
where A is a constant and the exponent A. is given explicitly by (4.4)
This can be expressed as the ratio of dimensionless logarithmic derivatives, namely A.
=
{[R ~ (In rcp)]/[R ~ (In boDd)]}. dR dR
(4.5)
R=Ro
It follows from eqs (4.2) and (4.3) that the curvature of the potential about equilibrium can be written as (4.6)
where n is the dimensionless logarithmic derivative of the bonding contribution to the potential. Hence, we have a normalized curvature about the
Structural stability: an illustrative example
79
equilibrium bond length R o that is given by , rep cxh
whereas the tetrahedron has J1.~
= 4(6)(h t )3 =  241ht l3 )
(4.56)
remembering that we can hop either clockwise or anticlockwise around a triangle. Hence, as is clear from Fig. 4.4, the eigenspectrum of the tetrahedron is more skewed than that of the rhombus. The eigenspectra are skewed downwards since J1.3 < O. Note that the eigenspectra in Fig. 4.4 have first been ordered from left to right according to whether the molecules are threedimensional, twodimensional, or onedimensional respectively. For a given dimension they are then ordered from left to right according to their degree of skewness, fi3/fi~/2, where fip = J1. p/J1.o' For threeatom molecules, the triangle and linear chain have a degree of skewness of 0.71 and 0 respectively. For fouratom molecules, the tetrahedron, rhombus, square, and linear chain have a degree of skewness of 1.16, 0.76,0, and 0 respectively (which follows directly from eqs (4.52), (4.55), and (4.56)). For fiveatom molecules, the trigonal bipyramid, monofinned tetrahedron, square pyramid, closepacked layer, pentagon, and linear chain have a degree of skewness of 1.23, 1.05, 0.85, 0.76,0, and 0 respectively. For sixatom molecules the trigonal tripyramid, octahedron, pentagonal pyramid, trigonal prism, closepacked layer, hexagon, and linear chain have a degree of skewness of 1.25, 1.00,  0.83,  0.39,  0.76, 0, and 0 respectively. Fourthly, counting all paths of length four within the linear chain, square, rhombus, and tetrahedron, we find
I
14 J1.7 4 
32 50 84
4
Ih 71
for)' =
s r
(4.57)
t
The different types of paths are shown in Fig. 4.7 for the tetrahedron. We see that per starting atomic site there are 3 twoatom paths, 12 threeatom paths, and 6 fourmembered ring paths, leading to a total of 4(3 + 12 + 6) = 84 paths per tetrahedral molecule as in eqn (4.57). The fourth moment measures the unimodal versus bimodal behaviour of the
94
Structure of molecules
3 twoatom paths
3 x 2 threeatom paths
Fig. 4.7 Examples of nearestneighbour paths of length four that contribute to the fourth moment of the tetrahedron's eigenspectrum. The solid atom indicates the site from which the path starts and to which it eventually returns. The number under each tetrahedron gives the total number of such paths starting and ending on the solid atom.
spectrum through a dimensionless shape parameter, s, namely S
= (A4/AD 
(AVA~)

(4.58)
1
where Ap = J1. p/J1.o. Us < 1, the spectrum is said to show bimodal behaviour, whereas if s > 1, it shows unimodal behaviour. The values of the normalized moments A2' A3' A4' and the shape parameters, s are given in Table 4.3 for the linear chain, square, rhombus, and tetrahedron. We see that the tetrahedron shows perfect bimodal behaviour with s = 0, corresponding to the eigenspectrum in Fig. 4.4, splitting into a deep singly degenerate bonding level and a triply degenerate antibonding level. The square, on the other hand, lies exactly on the unimodalbimodal borderline with s = 1, having Table 4.3 The normalized moments, A2 , A3' and A4' and the shape parameter, s, for the linear chain, square, rhombus, and tetrahedron (cf eqn (4.58». s t r
3 5/2
s
2
I
3/2
6 3
o o
o
21 25/2 8
53/125
7/2
5/9
1
Origin of structural trends: a moments theorem
95
its sizeable bondingantibonding level splitting neutralized by two nonbonding levels. The rhombus and linear chain take the values s = 0.424 and 0.555 respectively. We are now in a position to understand why the bond energy curves in Figs 4.5 and 4.6 cross each other. Let us first consider the relative stability of the two threeatom molecules, the linear chain and the triangle. Their eigenspectra have identical first three moments Ilo, Ilh and 112 for the case of ah = t corresponding to ..l = 2 (cf eqn (4.54», so that ~Ilp = 0 for P ~ 2. However, the eigenspectrum of the triangle is skewed downwards due to a negative third moment resulting from the threemembered ring contributions, whereas the linear chain's eigenspectrum is symmetric. Thus ~1l3 ~ O. This results in the twobond energy curves crossing once as a function of electron count as is seen in the upper lefthand panel of Fig. 4.5. Let us now consider the relative stability of the two fouratom clusters with symmetric eigenspectra, namely the linear chain and the square. Since 113 = 0, they have identical first four moments Ilo, Ill' 1l2' and 113 for ah = t, so that ~Ilp = 0 for P < 3. However, we see from Table 4.3 that ~1l4 ~ 0; the linear chain's eigenspectrum shows marked bimodal behaviour compared to that of the square. This is reflected in the eigenspectra in Fig. 4.4: the linear chain has a distinct bondingantibonding gap at the centre of the spectrum, whereas the square has a twofold degenerate nonbonding level exactly at the centre. Moreover, this increased weight at the centre of the square's eigenspectrum is compensated for by a wider overall spectrum than that of the linear chain, in order that their second moments remain identical. Thus, as the electron occupancy increases, we expect to find the structural trend from square . linear chain + square; that is, the two bond energy curves for the square and the linear chain will cross twice as a function of electron count, as is indeed observed in the middle lefthand panel of Fig. 4.5. In 1971 Ducastelle and CyrotLackmann proved a very important moments theorem that captures this crossing behaviour of the bond energy curves. Their moments theorem states that if two eigenspectra have moments that are identical up to some level Po, that is ~Ilp = 0 for P < Po, then the two bond energy curves must cross at least (Po  1)times as a function of electron count. Thus, we have seen in Fig. 4.5 that the triangle and the linear chain curves cross once, since Po = 2, whereas the square and the linear chain curves cross twice, since Po = 3. We can, therefore, understand the origin of the fouratom structural trend from tetrahedron . rhombus .linear chain . square as a function of the electron count for the case of ah = t. The presence of threemembered rings in a given geometry skews the eigenspectrum asymmetrically downwards. Hence, the closepacked structures, the tetrahedron and the rhombus, are stabilized for fractional electron occupancies less than onehalf but destabilized for fractional electron counts more than one half. On theother hand, the open structures, the square and the linear chain, have symmetric
96
Structure of molecules
eigenspectra. In addition, the linear chain has fewer paths of length four than the square, so that its eigenspectrum is more bimodal. Hence, the linear chain is stabilized for a fractional electron occupancy around onehalf but destabilized with respect to the square for fractional electron counts around threequarters or greater. We see from the middle panel of Fig. 4.5 that as the degree of normalized hardness increases from (til = t, the open structures become destabilized with respect to the closepacked structures until for (til = 1, corresponding to a hardcore potential, the linear chain is no longer found anywhere as a groundstate structure. This general feature of moving from closepacked to open structures as the electron count increases is displayed by the N = 3, 5, and 6 bond energy curves in Figs 4.5 and 4.6. We will see in Chapter 8 that the third moment skewing is also responsible for the observed trend from closepacked to open groundstate structure types across the spvalent elements within the periodic table. Further examples of the application of moments to understanding structural trends within molecules can be found in Burdett (1985) and Lee (1991).
4.6. The bond order The total bond energy of the molecule has been written as a sum over the occupied eigenvalues en' The eigenvalues (and eigenfunctions) are a global property of the molecule that results from diagonalizing the LCAO or TB secular equation. In practice, when comparing the bonding in molecules and solids, we would like to define a local bond energy between individual pairs of atoms. This can be achieved by decomposing the energy as follows: .AlVbond =
I L»; = If" n
=~ I,i
n
f
t/J(R) is a pairwise interatomic potential that represents the electrostatic interaction and overlap repulsion between neighbouring atoms. The second term F(Pi) is a manybody embedding potential that represents the ene~gy of embedding an atom at site i in the local charge density Pi which comes from the tails of the atomic charge clouds Patom on neighbouring sites j. The behaviour of the embedding function F(P) is illustrated in Fig. 5.16 for the case of hydrogen and the raregas atoms helium and neon. The curves were evaluated within the local density approximation (LDA) by embedding the atom in a homogeneous electron gas of density p. We see that He and Ne display a positive embedding energy at all densities because their closed electronic shells repel the free electron gas through orthogonality constraints. Moreover, the variation with density is linear so that from eqn (5.69) Fclosed(Pi)
= ap, = a I' Patom(Rij)
(5.70)
j
where a is an element dependent constant. Thus, the embedding function is pairwise and may be combined with the first contribution in eqn (5.68), leading to the wellknown result that the interaction between raregas atoms is accurately described by pair potentials. On the other hand, the openshell hydrogen atom shows a minimum in Fig. 5.16 at an attractive embedding
132
Bonding of spvalent metals
2.5 5 7.5 0.01
0.02
p{au~
Fig. 5.16 The embedding energy F(p) for H and the rare gas atoms He and Ne in a freeelectron gas of density p. (After Puska et al. (1981 ).)
energy of 1.8 eV. The shape of this embedding curve is well reproduced by adding an attractive square root dependent term to the repulsive linear term of the closedshell atoms, namely (5.71) where a and b are positive constants. The presence of this second term leads to the nonpairwise, manybody character of the embedding function in openshell systems. This nonpairwise behaviour is most easily demonstrated by considering the coordination number dependence of the binding energy. It follows from eqs (5.68), (5.69), and (5.70) that the binding energy per atom of a lattice with coordination number ,z may be written in the form
u = A~ 
B,zlf2
(5.72)
where A = ~(Ro)
+ apatom(R o)
(5.73)
and B
=
bp~~2m(Ro)
(5.74)
with R o being the nearest neighbour distance. Thus, if we plot the binding energy of different lattices with identical nearest neighbour distances R o as
Embedded atom potentials 133
o
E
+
1
E
.!!! ~

> 2 E'
a> c: W
+ 5 Coordination
10 ~
Fig. 5.17 The binding energy per atom U as a function of the coordination number ~ for aluminium. The crosses correspond to LOA predictions, whereas the curve is a leastsquares fit of the form of eqn (5.72). The lattice types considered are the linear chain (~= 2), graphite (~= 3), diamond (~= 4), twodimensional square mesh (~= 4), square bilayer (~= 5), simple cubic (~ = 6), triangular mesh (~ = 6), vacancy lattice (~ = 8) and face centred cubic (~ = 12). (After Heine et al. (1991).)
a function of coordination number ~ then we expect the results to fallon the curve given by eqn (5.72) since A and B will be constants. This is indeed the case for spvalent aluminium where we see in Fig. 5.17 that the predicted LDA values of the binding energy of different lattices with nearest neighbour distances equal to that of fcc follow the simple curve of eqn (5.72) surprisingly well. The squareroot dependence of the attractive contribution to the binding energy is a consequence of the unsaturated nature of the metallic bond. Hall the bonds were saturated then we would expect the binding energy to be directly proportional to the number of bonds present as the electrons in each bond would be localized between their parent atoms. However, in an spbonded metal there are not enough valence electrons to form saturated bonds with all close packed neighbours so that the electrons resonate between all bonds in a delocalized fashion. Increasing the local coordination about a given atom reduces the strength of neighbouring bonds as the electrons are spread more evenly between them. This is reflected in the fact that from eqn (5.72) the attractive binding energy per bond decreases as 1/~1/2 as the coordination number .e increases. This has important consequences for the energetics .of defects in metals. For example, the vacancy formation energy within a nearest neighbour pair
134
Bonding of spvalent metals
potential approximation is given by Au~:~r
=  .1:(R 0) + !~(Ro)
(5.75)
where the first term represents the loss in binding energy due to the breaking of ~ bonds when the atom is removed to create the vacancy, whereas the second term represents the energy gain equal to the cohesive energy Uco b when the removed atom is placed at the metal surface. We see, therefore, that a pair potential model predicts a vacancy formation energy equal to the cohesive energy, i.e. (5.76) This disagrees with experiment where the vacancy formation energy in metals is typically only about onehalf the cohesive energy. Using embedded atom potentials, however, there will be an additional lowering in the vacancy formation energy compared to that of pair potentials due to the fact that the .1: atoms surrounding the vacancy have one less neighbour and, therefore, experience a bond strengthening with their remaining (.1:  1) neighbours. This contributes an additional term (5.77) The prefactor outside the curly brackets gives the number of bonds that are strengthened by the absence of the atom at the vacancy site. The contribution inside the curly brackets gives the change in the bond energy due to the change in coordination from .1: to (.1:  1). For closepacked lattices .1:» 1 so that using the binomial expansion (5.78) where we have assumed that the cohesive energy is provided mainly by the attractive contribution  B.1: 1 / 2 in the binding energy. Thus, the embedded atom potential predicts the total vacancy formation energy (5.79) This is in good agreement with experiment. Em bedded atom potentials have been extensively used for performing atomistic simulations of point, line and planar defects in metals and alloys (e.g. Vitek and Srolovitz 1989). The pair potential (R), atomic charge density Patom(r), and embedding function F(P) are usually fitted to reproduce the known equilibrium atomic volume, elastic moduli, and ground state structure of the perfect defectfree lattice. However, the prediction of ground state structure, especially the competition between the common metallic structure types fcc, bee, and hcp, requires a more careful treatment of the pair potential contribution (R) than that provided by the semiempirical embedded atom potential. This is considered in the next chapter.
References
135
References Ashcroft, N. W. (1966). Physics Letters 23, 48. Ashcroft, N. W. and Mennin, N. D. (1976). Solid state physics. Holt, Rinehart and Winston, Philadelphia. Cohen, M. L. (1987). Microclusters (eds S. Sugano, Y. Nishina, and S. Ohnishi), page 2. Springer, Berlin. Daw, M. S. and Baskes, M. T. (1984). Physical Review B29, 6443. Finnis, M. W. and Sinclair, J. E. (1984). Philosophical Magazine ASO, 45. Gasiorowicz, S. (1974). Quantum physics. Wiley, New York. Girifalco, L. A. (1976). Acta Metallurqica 24~ 759. Heine, V. and Abarenkov, I. (1964). Philosophical Magazine 9, 451. Heine, V., Robertson, I. J., and Payne, M. C. (1991). Philosophical Transactions of the Royal Society (London) A334, 393. Herring, C. (1940). Physical Review 57, 1169. Jacobsen, K. W., Narskov, J. K., and Puska, M. J. (1987). Physical Review B35, 7423. Jan, J.·P. and Skriver, H. L. (1981). Journal of Physics Fll, 80S. Kittel, C. (1986). Introduction to solid state physics. Wiley, New York. Moruzzi, V. L., Janak, J. F., and Williams, A. R. (1978). Calculated electronic properties of metals. Pergamon, New York. Puska, M. J., Nieminen, R. M., and Manninen, M. (1981). Physical Review B24, 3037. Sutton, A. P. (1993). Electronic structure of materials. Oxford University Press. Tinkham, M. (1964). Group theory and quantum mechanics. McGraw·Hi1I, New York. Vitek, V. and Srolovitz, D. J. (eds) (1989). Atomistic simulations of materials: beyond pair potentials. Plenum, New York. Wigner, E. P. and Seitz, F. (1933). Physical Review 43, 804.
6 Structure of spvalent metals
6.1. Introduction The description of the metallic bond in the previous chapter assumed that the freeelectron gas remained homogeneously distributed as the pseudopotential lattice of ion cores was immersed within it. In practice, of course, the free electrons will respond to screen the ion cores, thereby leading to a modulation of the electron density. This modulated electron density then acts in turn on the underlying ionic lattice to give rise to a structuredependent contribution in the total energy. We will see in this chapter that this small structurally dependent contribution to the binding energy can be evaluated quantitatively using secondorder perturbation theory within the nearly free electron (NFE) approximation. Secondorder perturbation theory provides a reciprocal space representation of this structural energy, since it mixes together all plane wave states that are linked by the reciprocal lattice vectors of the underlying perturbing lattice. It is, therefore, the appropriate representation for describing those few NFE systems such as the HumeRothery electron phases that are stabilized in kspace by the unperturbed freeelectron Fermi sphere making contact with a zone boundary. More frequently, groundstate structural stability is determined by interaction between nearestneighbour shells of atoms in real space. The beauty of secondorder perturbation theory is that it also allows this structural energy to be written as a sum over oscillatory interatomic pair potentials. We will use this real space representation to provide an explanation for the structural trends within the spvalent metals that are observed in Table 1.1.
6.2. Screening: the ThomasFermi approximation Metals are characterized by an infinite static dielectric constant, so that any potential disturbance will be screened out by the electron response. This can be demonstrated most simply by considering a point ion of charge, Ze, immersed at the origin in a freeelectron gas of charge density  epo. The presence of the ion will induce a new electron density, p(r), which can be
Screening: the ThomasFermi approximation
137
related to the new potential, V(r), by Poisson's equation V2 V(r) = e2 [Zb(r)
+ Po 
p(r)]/eo·
(6.1)
The three contributions to the charge density on the righthand side are the positive charge Ze at the origin (represented by the delta function, b(r)), the compensating positive background charge, epo, ofjellium, and the perturbed electronic charge density,  ep(r). Note that strictly we should refer to V(r) as the potential energy, but we will maintain our previous custom and call V(r) the potential. In this chapter we will use atomic units throughout, so that e2 = 2, 4neo = 1, and 1l 2/2m = 1 (cf. Note on the choice of units, page (xi)). Hence, Poisson's equation can be written
v1 V(r) =
(6.2)
8n[Zb(r)  bp(r)] ,
where bp(r) is the induced change in electron density, namely bp(r)
= p(r)  Po.
(6.3)
We will solve eqn (6.2) within the ThomasFermi approximation by linking the change in electron density, bp(r), to the local potential, V(r). At equilibrium the chemical potential or Fermi energy must be constant everywhere as illustrated in Fig. 6.1, so that T(r) + V(r) = E~,
(6.4)
where T(r) and V(r) are the values of the kinetic and potential energies respectively at the position r. The term, E~, is the chemical potential of the undisturbed uniform electron gas of density Po, which from eqn (2.40) is E
'7lr)
EOF
r
Fig. 6.1 The localpotential energy, V(r), and local kinetic energy, T(r), such that the chemical potential is constant everywhere, taking the value ~.
138 Structure of spvalent metals given by
(6.5) The ThomasFermi approximation assumes the variation in the potential, V(r), to be sufficiently slow that the local kinetic energy, T(r), is equal to that of an homogeneous free electron gas with the same density p(r) as seen locally, that is
(6.6) Hence, using the binomial expansion and substituting eqn (6.6) into (6.4), we have E~[1
+ !bs(G).
(6.65)
G
This demonstrates immediately the importance of the location of the first few reciprocal lattice vectors with respect to the node at qo in the energywavenumber characteristic, 4'bs(q), which is illustrated in Fig. 6.6. Vectors lying at qo would contribute nothing to the bandstructure energy, which is consistent with zero band gaps opening up at the appropriate zone boundary. We found earlier that the G(I11) and G(200) reciprocal lattice vectors of aluminium lay just to the right of qo in Fig. 5.12, so that small negative contributions to the bandstructure energy in eqn (6.65) are obtained. However, on going down group III in the periodic table from Al + Ga + In we see from Table 6.2 that G(200) moves closer to qo and G(111), in fact,
150 Structure of spvalent metals Table 6.2 Values of Glqo for fcc aluminium, gallium, and indium. (From Heine and Weaire (1970) .)
G(111 )/qo G(200)/qo
AI
Ga
In
1.04 1.20
0.94 1.09
0.93 1.08
passes right through q0 to the other side. This is reflected by a change in the symmetry of the state at the bottom of the gap at L = (2rr:la) (1, 1, 1) on the Brillouin zone boundary. Whereas this state has the plike symmetry, L2" in aluminium (cf Fig 5.9), it has the slike symmetry, L 1 , in fcc gallium and indium. This behaviour in Glqo causes the reciprocal lattice vectors across the first Brillouin zone in fcc gallium and indium to lie closer to qo on average than those for fcc aluminium. It is, therefore, not implausible that the gallium and indium lattices distort from fcc in order to gain a marked lowering in their bandstructure energy as their distorted reciprocal lattice vectors move away on either side from the node at qo. A cubic to tetragonal distortion is illustrated schematically in Fig. 6.6, as is indeed observed for indium with
cia
=
1.08.
In practice, the degree of distortion is obtained by a balance between the electrostatic Madelung energy, which increases with distortion, and the bandstructure energy, which decreases with distortion. The realspace representation presented in the next section allows these two opposing contributions to be combined together into a single term, thereby facilitating an understanding of the observed structural trends within the elemental spvalent metals.
6.5. The realspace representation The total binding energy can be rewritten as a sum over real space rather than qspace vectors by changing the order of their summation in Ubs ' From eqn (6.57) the bandstructure energy is given by Ub s
= L S*(q)S(q)4>bs(q)  lim 4>bs(q),
(6.66)
4~O
4
where the q = 0 term has been included explicitly in the summation. Substituting in for the structure factor from eqn (6.47) and separating out the R, = Rj terms we have Ubs = _1_ L {~ L 4>bs(q) eiq.(Ri.Ri)} 2% j *j .;V 4
+ ~ L 4>bs(q) .;V
4
lim 4>bs(q). (6.67) 4
~0
The reelspace representation
151
This allows us to define the bandstructure contribution to a pair potential, namely (6.68)
Thus, we can write
The Madelung energy, eqn (6.61), can also be expressed as a pairwise sum over coulomb interactions between the point ions, plus a q + 0 contribution arising from the electronion and electronelectron interactions. Grouping this together with the bandstructure contribution we have Ubs + UMadelung _  1 "L.J (R i j ) 2% i *j
811:Z + ¥1>bs(R  0)  lim bs(q) + 1 2q + 0 2 q0 1
_
•
[
2
J ,
(6.70)
where the interatomic pair potential (R) is given by the sum of the ionion and bandstructure terms, namely (6.71)
In 1974 Finnis showed that the q + 0 limit could be evaluated directly by using the compressibility sum rule of the freeelectron gas, which relates the long wavelength behaviour of the dielectric constant to its compressibility. He found that
. [ lim bs(q) '1+0
811:Z + 1 ~2 2 q0
2J = 1Z 0 Beg + Ucore, 2
(6.72)
where Beg = Od 2 Ueg/d02 is the electrongas bulk modulus or inverse compressibility, and Ucore is the core contribution to the binding energy, eqn (6.61). Thus, the total binding energy per atom of a NFE metal can be expressed in a physically transparent form, as the sum of a volumedependent contribution and a pairpotential contribution in a manner that is reminiscent of the semiempirical embedded atom potential of eqn (5.68). It follows from eqs (6.59)(6.72) that (6.73)
where (6.74)
152 Structure of spvalent metals The electrongas term in eqn (6.74) is given from eqn (5.60) by Uel  fOBel = 0.982/r;  0.712/rs  (0.110  0.031 In rs)'
(6.75)
The bandstructure term is given from eqs (6.68) and (6.58) by rt>bs(R = 0) =
~2 [~ L OP(q)v~osn(q)J .At
(6.76)
q
as op(q) = x(q)vpiq). This contribution is, therefore, one half of the electrostatic interaction between an ion and its own screening cloud, so that it represents the binding energy of a screened pseudoatom. This expression is consistent with the virial theorem, where the equilibrium binding energy of all the electrons in a free atom is just one half of the total potential energy. It may be approximated by the simple expression (Finnis (1974)) rt>bs(R
= 0) ~
 Z2 qo/n
= !Z2/Rc
(6.77)
where the last equality holds for the Ashcroft emptycore pseudopotential from eqn (5.57). We see from Table 6.3 that eqn (6.77) reflects the large variation in the binding energy of the pseudoatoms in going across the period from Na + Mg + AI. The interatomic pair potential "'""II:.....C!"'""'.. cr §. ::;,
e
2 4
1
N
2
Fig. 6.16 Analysis of fcc, bee, and hcp relative structural stabilities within the rigidband approximation for CuZn alloys. (a) The difference in band energy as a function of band filling N with respect to elemental rigid copper bands. (b) The density of states at the Fermi level E F for fcc, bee, and hcp lattices as a function of band filling, N. (c) The difference in the Fermi energies AEF as a function of band filling, N. (After Paxton et al. (1992).)
170
Structure of spvalent metals
Further, it follows from eqs (6.111) and (6.112) that (6.114) Thus, the shape of the band energy difference curves in Fig. 6.16(a) can be understood in terms of the relative behaviour of the densities of states in the middle panel. In particular, from eqn (6.111), the stationary points in the upper curve correspond to band occupancies for which AEF vanishes in panel (c). Moreover, whether the stationary point is a local maximum or minimum depends on the relative values of the density of states at the Fermi level through eqn (6.113). Thus, the beefcc energy difference curve has a minimum around N = 1.6 where the bee density of states is lowest, whereas the hcpfcc curve has a minimum around N = 1.9, where the hcp density of states is lowest. The fcc structure is most stable around N = 1, where dE F ~ 0, and the fcc density of states is lowest. We see that the structural trend from fcc + bee + hcp is driven by the van Hove singularities in the densities of states. These arise whenever the band structure has zero slope as occurs at the bottom or top of the energy gaps at the Brillouin zone boundaries. The van Hove singularities at the bottom of the band gap at X and at the top of the band gap at L in fcc copper are marked X4 , and L 1 , respectively, in the middle panel of Fig. 6.16. It is, thus, not totally surprising that the reciprocalspace representation
4
i
bccfce(poly)
3
c:::
2
~ 1
a: E
5'Olwl!!I!fi~~~=Flc._
. ~
(I)
c
(I) 0)
c :ac m UAB(R/'S,
UA(ROA)
Nearest neighbour distance. R Fig. 7.14 The binding energy curves for the elemental A and B transition metals and the binary AB alloy. The heat offormation is given by AH= {JAB ~(UA + UB)' where the binding energies are evaluated at the appropriate equilibrium positions as shown.
This repulsive energy constraint implies from eqn (7.64) that the bond energy for the AB alloy must be evaluated for a value of ~B =
[!
>
E Q)
~
~ Q) c::::
Q)
c::::
Q)
Q)
"t:l
"t:l
m
m
c:::: 0
c:::: 0
?
?
?
? (4) ?
?
(1) (2) (3) (4) (3) (2) (1)
5
5 0
4 N
0
8
4 N
8
Fig. 8.2 The bond energy per atom of the fourfold, threefold, twofold and onefold coordinated lattices as a function of the number of valence electrons per atom, N, for the cases of degrees of normalized hardness of the potential, lI.h = 1 (lefthand panel) and lI.h = ; (righthand panel). The hard core potential of the lefthand panel cannot differentiate between different structure types for N > 5, whereas the realistic ':1. h =; potential gives the structural sequence for 4 + 3 + 2 + 1fold coordination of the (8N) rule. where the fraction of s admixture in the hybrid is 1/(1 + A. 2). Thus, sp, Sp2, and Sp3 hybrids correspond to A. = 1, and j3 respectively. The bond integral between these directed hybrids then takes the value,
fl,
h. = A
f
A.~i)fi A.~j) dr = sSO"  2A.spO"  A. 2 pp O" •
'Y A
'Y A
1 + A.2
(8.3)
This is plotted in Fig. 8.3 as a function of the percentage of s character, 100/(1 + A.2 ) , for two different choices of the ratios ppo rspc tssc, namely the solid curve where their magnitudes are all equal (cf eqn (3.58», and the dashed curve where their magnitudes are set according to Harrison's (1980) prescription for the bulk band structure (cf eqn (7.20». The full curve indeed predicts that Ihspl > Ihsp21> Ihsp31, which would drive the structural trend across the top panel of Fig. 8.1. Unfortunately, the more realistic dashed curve provides no such justification for the (8N) rule, since Ihspl < Ihsp21~ Ihsp31. In fact, the origin of the (8N) rule resides in the delicate balance between the repulsive overlap forces and the attractive covalent bond forces. The bond lengths are not invariant as drawn in Fig. 8.1, since the atoms do not behave as hard spheres with fixed nearestneighbour distances. Assuming a repulsive pair potential fI>(R)
= A[h(R)J2,
(8.4)
212
Structural trends within solids 4 PPpp and cI>dd respectively. It is a measure of the relative size of the p and d atoms as can be seen as follows. Consider a pair of transitionmetal atoms a distance 2R d = nlli apart. Then from eqs (8.45) and (8.46) a pair of metalloid atoms will show the same repulsive energy when they are separated by the distance 2R p such that (R p/R d )3 =
[it.
(8.51)
Thus, [it generalizes the concept of the relative size of hard spheres to the case where the mutual interaction varies smoothly rather than discontinuously.
Structural trends within the pdbonded AB compounds
235
The repulsive coefficients, (XII', depend only ·on structure and not on volume. They are given in Table 8.2, where the measured internal coordinates of MnP, FeB, CrB, and FeSi have been used to characterize the corresponding structure types. Two choices of the axial ratio, cia, have been chosen for the NiAs structure types; the first corresponds to the observed ratio of 1.39 for the NiAs compound, the second to the ideal ratio of (8/3)1/2. The repulsive potential in eqn (8.49) has been summed over the nearest neighbours only, other than for the pp coefficients of CsCI and FeSi, where further neighbours were included to generate better than 5% accuracy. The values of the repulsive coefficients in Table 8.2 reflect the local atomic environment. The metal (M) and metalloid (X) sites on the cF8 (NaCI) 6/6 lattice are both sixfold octahedrally coordinated with X and M atoms respectively, which form two interpenetrating cubic closepacked lattices. NaCI can, therefore, be described as a cubic closepacked arrangement of X atoms with all the octahedral holes occupied by M atoms. Structure type hP4 (NiAs) 81V/6', on the other hand, consists of a hexagonal closepacked arrangement of X atoms with the octahedral holes occupied by M atoms as shown in Fig. 1.10. The X sites are, thus, sixfold coordinated by a trigonal prism of M atoms, which themselves reside on a simple hexagonal lattice with eight nearest neighbours. The oP8 (MnP)10'"/8''' structure type is an orthorhombically distorted Table 8.2 The repulsive coefficients (XI/'. The number in brackets gives the number of atoms. included in the repulsive sum in eqn (8.49). (From Pettifor and Podloucky (1986).)
NaCI NiAs
(cia = 1.39) NiAs
(cia = 1.633)
MnP CsCI FeSi FeB CrB
ctpd
ctdd
ct p p
38.2 (6) 36.5 (6) 38.2 (6) 33.3 (6) 25.2 (8) 26.6 (7) 25.2 (7) 24.0 (7)
3.8 (12) 15.2 (8) 6.7 (8) 7.8 (8) 6.0 (6) 7.9 (6) 5.1 (10) 5.2 (10)
6.0 (12) 6.2 (12) 6.0 (12) 10.0 (12) 7.5 (6 + 12) 7.7 (6 + 12) 19.4 (10) 22.4 (10)
236
Structural trends within solids
variant of NiAs in which the X and M sites are surrounded by distorted trigonal prisms and octahedra respectively (cf. Fig. 1.9). The metal and metalloid sites on the cP2 (CsC!) 14/14 structure type are both surrounded by eight unlike atoms at the corners of a cube. The like atoms lie on a simple cubic lattice with six first and twelve secondnearest neighbours respectively. The cP8 (FeSi) 13'/13' structure type is related to CsCI but has seven nearest neighbours of opposite type instead of eight (cf. Fig. 1.9). The very similar oP8 (FeB) 17/9 and oC8 (CrB) 17/9 structure types are built up from zigzag chains of X atoms, which are surrounded by trigonal prisms of M atoms as shown in Fig. 1.12. The stacking together of these chains leads to an additional metal atom entering the coordination shell of the X site so that there are seven unlike nearest neighbours. The relative prepared volumes, which are required to satisfy the structural energy difference theorem, may be obtained from eqn (8.48) by setting AUr ep = O. The resultant firstorder change in volume An is given by (8.52) where the AiXll' are the corresponding changes in the repulsive coefficients. Therefore, the fractional change in volume is a function only of the relative size factor, gf, so that a universal curve may be plotted for each structure with a given set of internal coordinates. Figure 8.17 shows these curves with the CsCI lattice as reference, using the values of the repulsive coefficients in Table 8.2. As expected, the NaCI lattice has the smallest volume at either end of the [1t scale because, as C p or Cd tends to zero, the repulsion is dominated by one or other of the closepacked fcc sublattices. On the other hand, in the middle of the scale where the nearestneighbour pd repulsion dominates, the volume of the NaCI lattice with six nearest neighbours is about 13% larger than the CsCI with eight nearest neighbours. The packing of hard spheres would have predicted the much larger volume difference of 30%. The upper NiAs curve in Fig. 8.17, which corresponds to the observed axial ratio of 1.39 for NiAs, shows an increase in fractional volume with decreasing gf due to the large value of iX dd in Table 8.2. This arises from the strong dd repulsion within the chain of atoms lying along the caxis of the simple hexagonal metal sublattice. If the small Ni atoms are replaced by the larger transition metal atoms such as Ti or V from near the beginning of the series, then the axial ratio is observed to increase markedly in order to accommodate the increased dd repulsion. The lower NiAs curve is drawn for cia = 1.633, with this ideal axial ratio being adopted by MnTe. We see from Table 8.2 that iXdd now assumes a value more typical of the other structure types. The FeB, CrB curve in Fig. 8.17 is very strongly dependent on [1t as a result of the strong pp repulsion along the zigzag chains of p
Structural trends within the pdbonded AB compounds
237
tan1~
me . .
C'I
~
lij
~

a.'